Chemical Physics Letters 487 (2010) 77–80
Contents lists available at ScienceDirect
Chemical Physics Letters journal homepage: www.elsevier.com/locate/cplett
Photovoltaic properties of bisazomethine dye thin ﬁlms Takuya Hosokai a,*, Tetsuya Aoyama b, Takashi Kobayashi c, Aiko Nakao d, Shinya Matsumoto a,e a
Graduate School of Environment and Information Sciences, Yokohama National University, 79-2 Tokiwadai, Hodogaya-ku, Yokohama 240-8501, Japan Supramolecular Science Laboratory, RIKEN, 2-1 Hirosawa, Wako 351-0198, Japan c Faculty of Engineering, Osaka Prefecture University, 1-1 Gakuen-cho, Sakai 599-8531, Japan d Advanced Technology Support Division, RIKEN, 2-1 Hirosawa, Wako 351-0198, Japan e Faculty of Education and Human Sciences, Yokohama National University, 79-2 Tokiwadai, Hodogaya-ku, Yokohama 240-8501, Japan b
a r t i c l e
i n f o
Article history: Received 12 November 2009 In ﬁnal form 18 January 2010 Available online 21 January 2010
a b s t r a c t Photovoltaic properties of bisazomethine dye (DE2) in vacuum-deposited thin ﬁlms were examined for use in Schottky-type photovoltaic cells (ITO/DE2/Al). We measured dark and photo current–voltage characteristics and determined photocurrent action spectra. We conﬁrmed the p-type semiconductor property of DE2 thin ﬁlms evidenced by the formation of the Schottky barrier at the DE2/Al interface. We further found a relatively high incident photon to electron conversion efﬁciency comparable to that of metal phthalocyanine thin ﬁlms in devices having the same structure. These results demonstrate that DE2 thin ﬁlm is a candidate for a photocarrier-generating material in organic solar cells. Ó 2010 Elsevier B.V. All rights reserved.
1. Introduction Organic photovoltaic cells (OPVs) have attracted considerable attention because of their potential use in low-cost solar energy conversion, colourful and sophisticated design and device ﬂexibility [1–8]. In OPVs, organic thin ﬁlms sandwiched between a transparent conductive substrate and back electrode play a role in photocarrier generation. A strong extinction coefﬁcient in a wide optical range, especially in the visible range, is essential for organic thin ﬁlms to achieve high photocarrier generation efﬁciency. Optical properties of organic molecules, such as the optical gap and extinction coefﬁcient, can be tuned by designing the chemical structures and/or substituents. However, many signiﬁcant differences are often observed unexpectedly between the optical spectra of organic thin ﬁlms and the spectrum of a single molecule due to the coupling of molecular excitons among long-range molecules, molecular distortion, defects in a solid and so on [9–11]. Such difference between a solid and the component molecule is sometimes associated with an excellent materials property, and an organic photoconductor is a successful example. In this context, understanding the optical properties of organic thin ﬁlms is potentially of important for the promotion of OPVs as well as being of fundamental interest. N,N0 -bis[4-(N,N-diethylamino)benzylidene]diaminomaleonitrile (DE2), shown in Fig. 1, is a bisazomethine dye derived from diaminomaleonitrile together with 4-diethlaminobenzaldehyde and has
* Corresponding author. Present address: Institut für Angewandte Physik, Universität Tübingen, Auf der Morgenstelle 10, 72076 Tübingen, Germany. Fax: +49 7071 29 5110. E-mail address: [email protected]
(T. Hosokai). 0009-2614/$ - see front matter Ó 2010 Elsevier B.V. All rights reserved. doi:10.1016/j.cplett.2010.01.038
a high extinction coefﬁcient of 1.3 105 dm3 mol1 cm1 at 546 nm in chloroform . Because of its red ﬂuorescence in solution and in the solid state, DE2 has been examined as a ﬂuorescent material for organic light-emitting diodes . On the other hand, Matsumoto et al. reported that DE2 forms J-aggregates in vacuumdeposited thin ﬁlms of a speciﬁc thickness . J-aggregates are well known as photosensitizers in silver halide ﬁlms because of their sharp and narrow absorption band (J-band) . In addition to the above-mentioned properties, the large oscillator strength and fast electronic response of J-aggregates have attracted attention from the viewpoint of applications in various optoelectronic devices including OPVs [15–18]. However, the stability of conventional J-aggregates composed of an ionic dye in thin ﬁlms remains a practical problem. DE2 is a non-ionic dye, and thus, its J-aggregate thin ﬁlms are extremely stable. The absorption spectra of the J-aggregate thin ﬁlms do not signiﬁcantly change even after preservation for one year in ambient conditions or after thermal treatment at 373 K for 1 h . These points of interest have stimulated our study of DE2 thin ﬁlms. To date, we have reported the molecular arrangement in a single crystal, surface morphology and the electronic structure and photoluminescence properties of DE2 thin ﬁlms in detail [19–22]. In the present work, we study the photovoltaic properties of DE2 thin ﬁlms forming J-aggregates in Schottky-type cells. The simplicity of the device structure (i.e., electrode–organic thin ﬁlm–electrode) makes it a good starting point for evaluating the photovoltaic properties of organic materials. We show that the DE2 thin ﬁlms have p-type semiconductor properties and can be applied in Schottky-type solar cells. In addition, it is noted that the incident photon to collected electron efﬁciency (IPCE) is high and comparable to that reported for a similar primitive device
T. Hosokai et al. / Chemical Physics Letters 487 (2010) 77–80
(a) He I UPS DE2/ITO
N N Et = -C2H5
INTENSITY (arb. units)
Fig. 1. Chemical structure of DE2.
structure with metal phthalocyanine thin ﬁlms, suggesting that DE2 thin ﬁlms are strong candidates for photocarrier-generating materials in OPVs. 2. Experiment DE2 was synthesized according to Ref.  and puriﬁed using the recrystallization method. Photovoltaic cells were fabricated on indium tin oxide (ITO) substrates to produce a common sandwich structure. After cleaning the ITO substrates ultrasonically with pure water, 2-propanol, acetone and chloroform for 15 min consecutively and blow-drying them in nitrogen, the DE2 thin ﬁlm was prepared by vacuum deposition at a pressure of 3 104 Pa. The ﬁlm thickness (151 nm) was then determined using a surface proﬁler (Dektak IIA, Sloan). We note that the ﬁlm thickness gives rise to the formation of J-aggregates, as we reported previously . Finally, a semi-transparent Al electrode (0.28 cm2) was prepared using a metal shadow mask on the DE2 thin ﬁlm by vacuum deposition. We used a Keithley 6487 unit to measure the current–voltage (I–V) characteristics and short-circuit photocurrent. The light source was intensity-controlled monochromatic light from a tungsten lamp with a monochromator (CT-10, Jasco). Devices were illuminated through either the ITO electrode or Al electrode at an intensity of 5 lW cm2 to determine the IPCE spectra and photo I–V curve, where the transmittance of the Al electrode was taken into account so that the intensity at the surface of the DE2 thin ﬁlm was 5 lW cm2. All measurements were performed in an ambient atmosphere. He I ultraviolet photoelectron spectroscopy (UPS) was carried out using ESCALAB 250 (Thermo Fischer Scientiﬁc K.K.). DE2 thin ﬁlms with various thicknesses were prepared on a cleaned ITO substrate by the same procedure as that mentioned above. After breaking the vacuum, each sample was transferred immediately into the UPS apparatus. The samples were biased at 5 V during the measurement to obtain the cut-off position of UPS spectra.
KINETIC ENERGY (eV) (b) Energy level diagram EA: 3.3 eV 4.0 eV 1.9 eV 4.9 eV IP: 5.2 eV ITO
Fig. 2. (a) UPS spectrum of DE2 thin ﬁlms (thickness: 17 nm) on ITO substrate. (b) Energy level diagram of ITO/DE2/Al.
the preparation conditions, except substrate temperature, being signiﬁcantly different; i.e., in situ preparation under ultrahigh vacuum condition with very slow evaporation rate (0.2–0.3 Å/min). This suggests that the molecular orientation of DE2 thin ﬁlms is similar for the two deposition conditions and the molecules lie nearly ﬂat on ITO substrates independent of the ﬁlm thickness .
3. Results and discussion
Fig. 2a shows the typical UPS spectrum of DE2 thin ﬁlms on an ITO substrate. The ionization potential (IP) of DE2 thin ﬁlms was determined to be 5.2 eV by subtracting the energy width of the entire spectrum, which is the energy range from the onset to the cutoff position indicated in Fig. 2a, from the excitation source energy of 21.2 eV. Fig. 2b shows an energy level diagram of DE2 thin ﬁlms, where a measured work function (WF) of the ITO and a typical WF of Al electrode  are compared. The electron afﬁnity (EA) of 3.3 eV was obtained by subtracting the optical band gap of 1.9 eV for DE2 thin ﬁlm from the IP. According to the work by Kahn et al. , the IP and EA of DE2 thin ﬁlms are comparable to those of hexadecahydro metal phthalocyanine thin ﬁlms, which are typical p-type organic semiconductors used for OPVs. This could imply a p-type semiconductor property for the DE2 thin ﬁlms . It is worth noting that the UPS spectra determined here are quite similar to those determined by Hosokai et al.  despite
CURRENT DENSITY (A/cm2 )
3.1. Electronic structure of DE2 thin ﬁlm on ITO
3 x 10
2 x 10
1 x 10
Dark I-V characteristic ITO/DE2/Al
-1 x 10
VOLTAGE (V) Fig. 3. Dark I–V characteristic of ITO/DE2 (151 nm)/Al. The forward bias corresponds to the Al electrode being negative.
T. Hosokai et al. / Chemical Physics Letters 487 (2010) 77–80
3.2. Characterization of semiconducting properties and photocarrier generation of DE2 thin ﬁlm Fig. 3 shows the dark I–V characteristic for the ITO/DE2/Al device. The dark current signiﬁcantly increased at 1 V with forward bias, whereas the current did not change as greatly with reverse bias. This clear rectiﬁcation behavior demonstrates the semiconducting property of DE2 thin ﬁlms, which is presumably due to the Schottky barrier between DE2 and the Al electrode, considering the photocurrent action spectra presented below. We determined the short-circuit photocurrent action spectra for the ITO/DE2/Al device and calculated the external quantum efﬁciency (i.e., the IPCE) as
IPCE ð%Þ ¼ 124 jJsc j=ðk Ip Þ;
where Jsc (lA cm2) is the short-circuit photocurrent density and k (nm) and Ip (mW cm2) are the wavelength and intensity of the incident light, respectively. Fig. 4a shows the IPCE spectra of ITO/ DE2/Al under illumination through the Al and ITO electrodes (IPCEAl and IPCEITO spectra). For a comparison of the IPCE spectra, absorption spectra of DE2 thin ﬁlms with a thickness of 151 and 60 nm are shown in Fig. 4b. As reported previously , the sharp peak at 641 nm in the absorption spectrum of the 151 nm-thick ﬁlm has been characterized as the J-band, while the spectrum of the 60 nm-thick ﬁlm has no such a J-band, showing there is no J-aggregates in the ﬁlm. Short-circuit photocurrent was observed in a primitive device structure of ITO/DE2/Al. This demonstrates that
WAVELENGTH (nm) 300 4
from Al from ITO
(b) OPTICAL DENSITY
151 nm 60 nm
DE2 thin ﬁlms can generate and transport photocarriers in photovoltaic cells. IPCE spectra were dependent on the direction of illumination. We observed higher IPCE throughout the measurement region by illuminating through the Al electrode. This result was valid even if a small absorption of the ITO in the visible region was taken into account for the IPCEITO spectrum. These results suggest that a Schottky barrier is formed at the interface between DE2 and the Al electrode. We note that the IPCE of a few percent in the IPCEAl spectrum (e.g., 2.7% at 564 nm) is comparable to that for traditional photovoltaic cells with metal phthalocyanine thin ﬁlms in a similar primitive device structure [25,26]. In general, the Schottky barrier region in Schottky-type OPVs is thought to be limited to the interface between organic thin ﬁlms and an electrode or within a thickness of several monolayers from the interface. Therefore, IPCE depends on the number of incident photons (or excitons) reaching to the Schottky barrier region through the organic thin ﬁlms or an electrode. For a case of the DE2 device structure, under illumination through the Al electrode incident photons are absorbed at the interface (i.e., the Schottky barrier region), and thus, photocarriers are efﬁciently generated. On the other hand, under illumination through the ITO electrode, photocarrier generation is limited because quite less incident photons can reach to the DE2/Al interface in the measurement region of the IPCE spectra due to the strong absorption of the DE2 thin ﬁlm (see Fig. 4b). This phenomenon results in the different spectral shape for IPCEAl and IPCEITO spectra and is the so-called ﬁltering effect that is often observed in Schottky-type photovoltaic cells [27– 30]. As a consequence, the IPCEAl spectrum matches the absorption spectrum (the symbatic response) except for the J-band at 641 nm, whereas the IPCEITO spectrum is more concave (the antibatic response). Although the reason why no clear contribution of the Jband was observed in the IPCE spectra has not yet been clariﬁed, the excitons of the J-aggregates might not contribute to the photocarriers generation in this device conﬁguration or the density of Jaggregates might be very low. Although one might suspect that the peak at 640 nm in the IPCEITO spectra could be assigned to the contribution of the J-band, we conﬁrmed that the peak is derived from the ﬁltering effect by comparing the absorption spectra of the Jaggregate thin ﬁlm and the non J-aggregate thin ﬁlm shown in Fig. 4b and the IPCE spectra . It is worth noting that a previous study showed that excited J-aggregates transfer energy to the metal electrode efﬁciently through the excitation of surface plasmon, and thus, the contribution of J-aggregates to the IPCE appears to decrease . Such non-radiative decay of excited J-aggregates can be prevented by the insertion of a C60 layer between J-aggregates and the metal electrode . To prevent the non-radiative decay, we also constructed heterojunction devices of ITO/DE2/ C60/Al and determined the IPCE spectra. The IPCE increased to 14.0% at 548 nm for IPCEAl spectrum because of an efﬁcient charge separation at the donar (DE2)/acceptor (C60) interface. However, a clear contribution of the J-band was not observed in the IPCE spectra. These results for the heterojunction devices will be discussed in detail elsewhere. 3.3. Characterization of photovoltaic properties of DE2 thin ﬁlm
1 0.5 0 300
WAVELENGTH (nm) Fig. 4. (a) IPCE spectra of ITO/DE2 (151 nm)/Al illuminated through the Al or ITO electrode. (b) Absorption spectra of the DE2 thin ﬁlms with a thickness of 151 nm and 60 nm.
Fig. 5 shows the photo I–V characteristic of ITO/DE2/Al illuminated with 600 nm monochromatic light through the Al electrode, where the dark I–V characteristic depicted in Fig. 3 is also shown for a comparison. Several fundamental parameters such as the open circuit voltage (Voc), ﬁll factor (FF) and Jsc can be extracted from the photo I–V curve. FF is deﬁned as the maximum power output of the cell divided by the product of Voc and Jsc. Under this measurement condition, we obtained Voc = 1.06 V, Jsc = 6.47 105 mA cm2 and FF = 0.28. The observed value of Voc is slightly
T. Hosokai et al. / Chemical Physics Letters 487 (2010) 77–80
CURRENT DENSITY (nA cm )
Part of this work was supported by the Industrial Research Grant Program of the New Energy and Industrial Technology Development Organization (NEDO) of Japan. The authors are grateful to Dr. T. Tanaka (Sumitomo Chemical Co. Ltd.) for helpful discussions.
     
 Fig. 5. Photo and dark I–V characteristic of ITO/DE2 (151 nm)/Al. The photo I–V characteristic was determined by illuminating a monochromatic light of 600 nm with an intensity of 5 lW cm2 at DE2/Al interface through the Al electrode.
higher than that for a metal phthalocyanine thin ﬁlm having the same device structure [25,26,33]. A similar value of FF is frequently obtained for Schottky-type OPVs due to high series resistance (Rs) of organic thin ﬁlms [34,35]. For the photo I–V curve, the higher current density above the Voc and the continuous change in the current in the third quadrant can be ascribed to the decreasing of the Rs due to the photoconductivity of the DE2 thin ﬁlm by light illumination. The power conversion efﬁciency of a photovoltaic cell (g) is given by
g ð%Þ ¼ ðjJsc V oc j=Io FFÞ 100;
             
where Io = 5 lW cm is the incident light power in this measurement. The efﬁciency g was estimated to be 0.38%. In general, the efﬁciency g of a Schottky-type OPV depends largely on the intensity of the incident light, surface treatment of the substrate, cell area and other considerations. Nevertheless, the observed efﬁciency g of the DE2 cell is comparable to values for ITO/ metal phthalocyanine/Al devices reported in the literature [25,26], for which the measurement conditions were similar to those in this study. Although optimization of the DE2 device possibly improves the efﬁciency g , the observed efﬁciency g indicates that DE2 thin ﬁlms can be used in OPVs as an active layer.
         
4. Conclusions We studied the photovoltaic properties of DE2 thin ﬁlms forming J-aggregates in a Schottky-type cell. It was revealed that the DE2 thin ﬁlms form a Schottky barrier at the interface with the Al electrode and work as a p-type semiconductor. Although we did not ﬁnd an apparent contribution of J-aggregates in the photocurrent action spectra, we observed IPCE comparable to that of metal phthalocyanine thin ﬁlms. These results indicate that ITO/DE2/ Al devices can be applied in Schottky-type solar cells and that a DE2 thin ﬁlm is a candidate for a photocarrier-generating material in OPVs.
   
C.W. Tang, Appl. Phys. Lett. 48 (1986) 183. G. Yu, J. Gao, J.C. Hummelen, F. Wudl, A.J. Heeger, Science 270 (1995) 1789. J. Xue, S. Uchida, B.P. Rand, S.R. Forrest, Appl. Phys. Lett. 84 (2004) 3031. S. Günes, H. Neugebauer, N.S. Sariciftci, Chem. Rev. 107 (2007) 1324. C.J. Brabec, Sol. Energy Mater. Sol. Cells 83 (2004) 273. B.P. Rand, J. Genoe, P. Heremans, J. Poortmans, Prog. Photovolt.: Res. Appl. 15 (2007) 659. K. Suemori, T. Miyata, M. Yokoyama, M. Hiramoto, Appl. Phys. Lett. 85 (2004) 6269. T. Taima, M. Chikamatsu, Y. Yoshida, K. Saito, K. Yase, Appl. Phys. Lett. 85 (2004) 6412. M. Kasha, H.R. Rawls, M.A. El-Bayoumi, Pure Appl. Chem. 11 (1965) 371. J. Mizuguchi, G. Rihs, H.R. Karfunkel, J. Phys. Chem. 99 (1995) 16217. U. Heinemeyer, R. Scholz, L. Gisslén, M.I. Alonso, J.O. Ossó, M. Garriga, A. Hinderhofer, et al., Phys. Rev. B 78 (2008) 085210. R.W. Begland, Preparation of disperse bisanil dyes derived from diaminomaleonitrile, US Patent 3962220, 1976. J. Yu, Z. Chen, M. Sone, S. Miyata, M. Li, T. Watanabe, Jpn. J. Appl. Phys. 40 (2001) 3201. S. Matsumoto, T. Kobayashi, T. Aoyama, T. Wada, Chem. Commun. (2003) 1910. T. Kobayashi, J-Aggregates, World Scientiﬁc Publishing Co. Pte. Ltd., 1996. K. Saito, Jpn. J. Appl. Phys. 38 (1999) L1140. M. Kawasaki, S. Aoyama, Chem. Commun. (2004) 988. M. Era, C. Adachi, T. Tsutsui, S. Saito, Chem. Phys. Lett. 178 (1991) 488. S. Matsumoto, K. Shirai, K. Kobayashi, T. Wada, M. Shiro, Z. Kristallogr. 219 (2004) 239. T. Hosokai, S. Kera, S. Matsumoto, K.K. Okudaira, N. Ueno, Mol. Cryst. Liq. Cryst. 472 (2007) 43. T. Kobayashi, S. Masumoto, T. Tanaka, H. Kunugita, K. Ema, T. Aoyama, T. Wada, Phys. Chem. Chem. Phys. 7 (2005) 1726. S. Matsumoto, M. Satoh, D. Tsuchida, T. Kobayashi, T. Aoyama, T. Wada, Trans. MRS J. 30 (2005) 345. K. Shirai, M. Matsuoka, K. Fukunishi, Dyes Pigm. 47 (2000) 107. A. Kahn, N. Koch, W. Gao, J. Polym. Sci. Polym. Phys. 41 (2003) 2529. T. Iwase, Y. Haga, Jpn. J. Appl. Phys. Part 1 42 (2003) 5330. H. Yonehara, C. Pac, Thin Solid Films 278 (1996) 108. R.O. Loutfy, J.H. Sharp, C.K. Hisao, R. Ho, J. Appl. Phys. 52 (1981) 5218. A.K. Ghosh, T. Feng, J. Appl. Phys. 49 (1978) 5982. M.G. Harrison, J. Grüner, G.C. Spencer, Phys. Rev. B 55 (1997) 7831. T. Stübinger, W. Brütting, J. Appl. Phys. 90 (2001) 3632. It has been considered by a thickness dependence of optical spectra  and a study of surface morphology  that the J-aggregates of DE2 molecules exist at a surface but not in a bulk region of the ﬁlms. According to Ghosh and Feng , an absorption spectrum of a bulk region which induces a ﬁltering effect in photocurrent action spectra can be approximately calculated by a following relation, IPCEAl/IPCEITO. For the case of our Schottky cell, the calculated absorption spectrum does not match the absorption spectrum of the Jaggregate thin ﬁlm (thickness: 151 nm) but can match the non-J-aggregate thin ﬁlm (thickness: 60 nm) shown in Fig. 4b. Therefore, we can suggest that the peak at 640 nm in the IPCEITO spectrum originates from the ﬁltering effect due to the absorption in the bulk region of DE2 thin ﬁlms without J-aggregates. K. Saito, J. Phys. Chem. B 103 (1999) 6579. C.Y. Kwong, A.B. Djurišicˆ, P.C. Chui, L.S.M. Lam, W.K. Chan, Appl. Phys. A 77 (2003) 555, and references therein. T. Aernouts, W. Geens, J. Poortmans, P. Heremans, S. Borghs, R. Mertens, Thin Solid Films 403–404 (2002) 297. S. Uchida, J. Xue, B.P. Rand, S.R. Forrest, Appl. Phys. Lett. 84 (2004) 4218.